Loading in 2 Seconds...
Loading in 2 Seconds...
The Low Temperature Magnetic Properties of Bulk and Nanoparticle DPPH. Donovan L. Thompson, a,b Yitzi M. Calm, a,b Fabrizio Guzzetta, c Ou Chen, c Y. Charles Cao, c Alexander Angerhofer, b,c and Mark W. Meisel a,b
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
of Bulk and Nanoparticle DPPH
Donovan L. Thompson,a,b Yitzi M. Calm,a,b Fabrizio Guzzetta,c Ou Chen,c Y. Charles Cao,c Alexander Angerhofer,b,c and Mark W. Meisela,b
aDepartment of Physics, University of Florida, Gainesville, Florida 32611-8440
bNational High Magnetic Field Laboratory (NHMFL), Gainesville, Fla 32611-8440
cDepartment of Chemistry, University of Florida, Gainesville, Florida 32611-7200
The magnetization of bulk and nanoparticle samples of DPPH
[2,2-Diphenyl-1-Picrylhydrazyl] have been measured from 2 K to 300 K in magnetic fields of 100 G. At 2 K, isothermal magnetization studies were performed in fields up to 70 kG. The data and analysis suggest unusual magnetic behavior exists below ~ 15 K. At higher temperatures, the results can be explained by weakly or non-interacting magnetic spins.
There were two ways used to load DPPH samples for magnetization measurements: in a “can”, and sample in a “gelcap”. The can is a 0.273 mL polyethylene container with a cover that latches. The gelpcap is a gelatin ~ 0.2 mL capsule. The sample was loaded into its container, which was mounted into a drinking straw that moved through the pickup coils in the magnetometer. First, the sample was centered at (300 K, 0 G) and then centered at (300 K, 100 G) and (300 K, 3 kG).The magnetic properties were studied as a function of temperature, down to T = 2 K, and magnetic field, up to H = 70 kG, by using a Quantum Design magnetic properties measurement system (MPMS). The sample masses were recorded using a Mettler AE163 analytical balance. The molecular weight of DPPH is 394.32 g/ mol.
The bulk DPPH sample was purchased from Sigma-Aldrich (1898-66-4) and used without further purification.
DPPH was recrystallized twice from carbon disulfide (CS2). Typical crystallites were needles of 1 to 2 mm length and 0.1 to 0.2 mm thicken.
Synthesis of DPPH (NPs):
First, DPPH (11 g) was dissolved in THF
(2 ml) under Ar to form a deep purple colored stock solution, of which 100 µl was injected into a flask with 5 ml of water (Nanopure, 18.2 MΩ) at room temperature with vigorous stirring. After a predetermined growth time (0-2 h), aqueous gelatin solution (1.8 ml, 2 wt %) was injected into the growth solution, which was kept under stirring for 5 more minutes; the DPPH NPs were then isolated from the growth solution through centrifugation at 15,000 rpm and 20o C .
The free organic radical DPPH in its bulk form with one unpaired electron per molecule (S = 1/2) has been investigated for a long time in many research laboratories [1-4]. The molecule is of interest because of widespread use in EPR (Electron Paramagnetic Resonance) due to its single, narrow resonance line that is used for g-factor determination and magnetic scan calibration . The motivation of this research is to characterize the low temperature magnetic response of nanoparticles (NPs) of DPPH and to contrast those results with the behavior of their bulk counterparts.
Fig. 1. The temperature dependence of the magnetic susceptibilities in zero field cooled with a constant field of 100 G (bulk) and 3 kG (crystals). The inset shows susceptibilities of field cooled minus zero field cooled.
Fig. 2. Zero- field cooled susceptibility- temperature product versus temperature of DPPH with a constant field of 100 G (Bulk) and 3 kG (crystals).
DPPH (NPs) will be tested using the SQUID Magnetic Property Measurement System (MPMS) and additional susceptibility measurements are needed to help clarify these interpretations.
Fig. 3. Zero- field cooled temperature dependence of the susceptibility reciprocal with a constant field of 100 G (Bulk) and 3 kG (crystals).
DPPH EPR measurements:
This work has been supported, in part, by the National Science Foundation via the NHMFL REU Program, the UF Department of Physics REU,
DMR-0701400 (MWM), CHE-0809725 (AA), and DMR-0645520 (YCC).
 W.Duffy and K. Barr, Phys. Rev. 165, 654 (1968).
 O.Chen, J. Zhuang, F. Guzzetta, J. Lynch, A. Angerhofer, and Y. Cao, J. Am. Chem. Soc. 131, 12542 (2009).
 P. Grobet, L. Gerven, and A. Bosch, J. Chem. Phys. 68, 11 (1978).
 K. Mukai, K. Nedachi, J. Jamali, and N. Achiwa, Chem. Phys Letters. 214, 560 (1993).
Fig. 4. The field (H) dependence of the magnetization (M) was measured at 2 K.
Fig. 6. NP EPR line width (LW) versus temperature inverse .
Fig. 5. EPR spectrum of 250 nm DPPH NPs (9.5 GHz).